PrefacePaint has been used for artwork for many thousands of years. The oldest Mediterraneancivilizations including the Greeks, Romans, and Egyptians used encaustics, paintsmade with a mixture of mineral pigments (iron, copper, manganese oxides, etc.),melted beeswax, and resin and then ﬁxed with heat. Tempera, a ﬂuid mixture ofbinder (organic medium), water, and volatile additives (vegetal essential oils) andorganic binders made of materials available from animal sources (whole egg, animalglues, or milk) were used to make paints for hundreds of years. At the end of the Roman Empire and up to the Renaissance period (ﬁfteenthcentury), these ancient formulas were lost and replaced by oil paint and/or tempera.In Italy and Greece, olive oil was used to prepare pigment mixtures, but the dryingtime was excessively long and unpredictable. Gradually, paints were reﬁned withdifferent oils and additives, working in combination with heat, to produce a group ofreliable resin systems and solvent blends for modern industrial coatings that providethe appearance characteristics to satisfy consumers and protective characteristics tomake the product last in different environments and conditions. Modern coatings arenow used on virtually every durable-good product manufactured. In more recent history, the need to clean up the environment has had a profoundimpact on coating formulation. Higher solids content and water content have changedto reduce the solvent included in the blend and reduce waste and emissions generatedby the use of surface coatings. Surface coatings are used on furniture, toys, automobiles, bicycles, computercabinets, televisions, and thousands of other products. Many of these products arecoated with liquid organic paints. Paint provides a decorative or protective coatingon a metal, plastic, or wood product. Paint is also applied for insulation, to reﬂectlight, or conduct electricity. The average person can see the decorative value of paint, and many products arepurchased because of eye appeal. Although it is less obvious at the time of purchase,resistance to the elements is equally important, and consumers appreciate the fact thatthe products they own will stay cleaner, last longer, and resist corrosion because theyare protected by a high-quality industrial coating. xiii
AuthorRodger Talbert is an independent consultant working in surface ﬁnishingtechnology. He designs new systems for liquid spray coating, powder coating,and electrodeposition, and works to improve existing systems through processimprovement, retroﬁt, and training. Talbert began his career in coatings in 1976, working for a company involvedin custom coating and metal fabrication. He also worked 7 years for a companythat designs and builds coating systems. He started his own business, R. TalbertConsulting, Inc., in 1993. Talbert has taught Powder Coating and Finishing System Design and Operation atGrand Rapids Community College, where he designed and implemented a FinishingTechnician Certiﬁcate program and published six training manuals for liquid coating,electrocoating, and powder coating classes. He is the editor of The Powder Coater’sManual, and he is a member of the technical advisory committee for the Iowa WasteReduction Center. He also conducts periodic training workshops in liquid coatingspray technique, powder coating, and systems design. Talbert received his education in business administration at Aquinas College inGrand Rapids, Michigan. He is a member of the Powder Coating Institute (PCI)and a member of the Electrocoat Association. He is the former chairman of theApplication & Recovery Committee of the PCI, chairman of education for ChemicalCoaters Association (CCAI), technical director for CCAI, and former president of theNational Board of Directors for CCAI. He has written and presented numerous technical papers for SME/AFP, PCI, andCCAI. He has contributed to the SME Design for Manufacturing handbook on thesubject of powder coating, is a contributor to the PCI Powder Coating Terms &Deﬁnitions handbook, and is a contributor to the PCI Powder Coating Manual andThe Complete Finishers Handbook. He also wrote the chapter on powder coating inthe Manufacturers Engineering Handbook, published by McGraw-Hill. xv
1 Part Preparation Processes and EquipmentA coating is applied to a part to enhance its appearance and to protect the substratematerial. An organic coating will act as a physical barrier to moisture, but if thecoating surface is damaged, the bare metal is exposed, and corrosion can form andspread. The adhesion of the coating and the corrosion resistance of the productdepend on the preparation of the surface. Part preparation is often referred to aspretreatment. The term pretreatment is used to deﬁne the mechanical or chemical surfacetreatment for a manufactured product, referred to as the substrate, to clean it, andprepare it for the application of a coating. Pretreatment can be accomplished in manydifferent ways. For example, sanding a part to remove dirt is a simple mechanicalmethod of part preparation. Chemical pretreatment may be as simple as a solvent wipe,or it may be a multistage spray washer that cleans the part and applies a conversioncoating. The speciﬁc method and degree of pretreatment used depends on qualityrequirements of the product. Pretreatment typically provides better adhesion of the coating to the part and helpsprevent the spread of corrosion, adding value to a product and extending its useful life.Pretreatment eliminates reactions between metals and between coatings and metals.It also cushions expansion and contraction differences between the substrate and thecoating. Pretreatment is one of the most important steps in ensuring that the coating willperform as intended. A decorative coating will not hide defects, and the performanceof a coating is directly related to the condition of the surface that it is applied to.Application of the coating over a contaminant will prevent it from forming a tightbond to the substrate, and if the contaminant lifts off, so will the coating. Dirt particleswill not dissolve or be hidden by the coating. For good appearance and adhesion,the part must be clean. In addition to cleaning, it may be necessary to develop a conversion coatingon metal surfaces prior to coating application. With the exception of some preciousmetals such as silver, gold, and platinum, metals react with air to form an oxide layeron their surface. Water molecules are tightly held to this oxide layer. This is not agood surface condition for chemical bonding. An example of a surface that has beentreated with a conversion coating is shown in Figure 1.1. Deciding what process can be used to pretreat a particular part depends on theperformance requirements of the ﬁnal part, pretreatment requirements of the paintto be used, the substrate material, and soils on the surface. 1
2 Paint Technology HandbookFIGURE 1.1 Magniﬁed zinc phosphate surface.1.1 CLEANINGManufactured products have a variety of contaminants on their surfaces. Before acoating is applied to the substrate, the surface has to have these contaminants removed.If contamination is left on the surface, the coating may not meet the required qualitystandards for appearance, adhesion, or corrosion resistance. The kind of pretreatment to use will depend on the types of soil found on thesurface and the quality goals for the product. A good deﬁnition of the level of per-formance that is required will lead to a cleaning process that is effective and reasonablein cost.1.1.1 TYPES OF SOILRaw materials that are stored, handled, or used for manufacturing products willalways have some surface contamination. On metals, the probable contaminantsare oily soils, including petroleum products, animal fat, or vegetable oils depos-ited during manufacturing operations for rust protection, drawing, machining, andforming. There may also be heavy-duty drawing compounds and lubrication greases orwaxes and some solid soils such as carbon, graphite smuts, metal shavings, polishingproducts, metal oxides, welding scale, and rust or corrosion. Plastics may have mold release, skin oils from handling, plastic particles fromsanding, and dust and dirt from the atmosphere. There are a variety of mechanical and chemical methods that can be used toclean metals and plastics. Accurate identiﬁcation of soils leads to the proper cleanerselection and helps verify cleanliness. The ﬁrst step is to do a soil audit to determinewhat types of soils will need to be removed.
Part Preparation Processes and Equipment 184.108.40.206 Rust InhibitorsLubricants, parafﬁn waxes, oils, drawing compounds, and similar rust inhibitorsare made from petroleum oils. Oils will usually break down pretty well in alkalinechemical cleaners.220.127.116.11 Shop DirtDust, shop dirt, and other forms of particulate can be removed with most alkaline oracidic cleaners and can also be removed by mechanical blasting or grinding, followedby a blow off.18.104.22.168 CarbonCarbon is present in all organic compounds and in a few inorganic compounds. It isabundant in various steel alloys in the form of metal smut. Carbon smut is extremelyinert and nonreactive due to electrostatic attraction to metal surfaces. Chelants do avery good job of breaking down smut whereas alkalis, solvents, and most acids arenot very effective. Mechanical cleaning can also be very effective at removing smutfrom a steel surface.22.214.171.124 OxidationAn oxide of any metal can develop on the metal surface right after the metal isformed or cast. Aluminum oxide and zinc oxides are white, while iron oxide is redrust. Copper oxide is recognized as a green tarnish. Acids are extremely good forthe removal of oxides since all oxides are acid soluble. Some alkaline products thatare not inhibited will remove zinc and aluminum oxides. Solvents are typically noteffective. Mechanical cleaning is very effective for the removal of oxide layers. Laser cutting is a commonly used process for many different gauges of steel.The laser cutting process creates an oxide layer on the edge that has been cut. Paintwill adhere to the laser oxide but the laser oxide is not tightly adhered to the steel.If the coating is cracked along the edge it may completely delaminate, especiallyif the product is used out-of-doors. Sanding, grinding, chipping, and blasting can be very effective for the removalof laser scale. Hand methods are somewhat limited due to the high labor content andthe inherent inconsistencies associated with manual operations. Some shapes may bedifﬁcult to clean by hand. Automated blasting can be very effective if the steel is heavy enough to withstandthe pressure and all surfaces are accessible to the blast media. Blasting may be agood way to treat laser edge when hot-rolled steel (HRS) is used because the scaleand other inorganic soils can also be removed. Acidic chemical solutions have also been effectively used for the removal oflaser oxide. Many of these solutions are phosphoric acid-based solutions applied byspray or in immersion systems. Phosphoric acid is aggressive enough for the taskwithout over-reaction that may occur with some other acids.
4 Paint Technology Handbook The disadvantage of phosphoric acid is the signiﬁcant volume of iron phosphatesludge, which, over time, without proper circulation and ﬁltration, builds up in thetank, fouling heat exchangers, clogging plumbing systems, and eventually resultingin expensive system cleaning and downtime. In addition, in some cases, the strongacid solution will leave ﬁne metal particles on the surface that show up in the coating. In some instances, blends of acids are the most effective chemical approach. Thereare commercially available blends of acids that work synergistically to remove laserscale without many of the negative aspects of a single acid. In addition to selectingthe proper chemistry, you must also apply the product properly. Adjusting cleanerconcentration and bath temperature can optimize cleaning time. It is very important to involve the chemical supplier for a wash system to makesure that the design for chemical removal of laser scale considers the compatibility ofall the system chemistry with the process equipment’s material of construction. Laserscale can be effectively removed when necessary using acid-resistant equipment andblended engineered chemicals.126.96.36.199 WaxWaxes are similar in composition to fats and oils. Some are hydrocarbons, whileothers are esters of fatty acids. They are water repellent, nontoxic, smooth textured,and resistant to many chemical cleaning products. Waxes are often used on tubingas a rust inhibitor. They are solids at ambient temperatures so the cleaner used mustreach the melting point of the wax to break it down. They are soluble in most organicsolvents and alkaline cleaners, providing that the contact time is long enough and thetemperature is high enough.188.8.131.52 SoapsSoaps are sometimes formed by the water-soluble reaction of a fatty acid andan alkali. Soaps lower the surface tension of water and permit emulsiﬁcation of fatbearing soils. Soft soaps, heavy metal soaps, and vegetable oil soaps can be foundin products such as metalworking ﬂuids. Alkaline cleaners are generally the best atsaponifying soaps. Acids will turn the soap to a semisolid mass and make rinsing moredifﬁcult. Solvents are usually not effective, too expensive, and not environmentallydesirable.184.108.40.206 PolymersPolymers are sometimes used in compounds to provide good lubricity and releasingproperties during certain manufacturing processes. Organic polymers can be natural,synthetic, and semisynthetic molecules such as phenolic materials and celluloses.Inorganic materials include siloxanes, silicones, and sulfurized polymers. Acids,alkaline cleaners, solvents, and detergents can be used to remove polymers.220.127.116.11 SiliconeSilicones are sometimes used as lubricants or release agents in manufacturing pro-cesses. Silicones can be liquid, solid, or semisolid. These are long, straight-chain
Part Preparation Processes and Equipment 5polymers, very low in surface tension, and they are not easily broken down usingalkaline or acidic products. They can be removed with organic solvents, but thesolvent will become contaminated very quickly.1.1.2 MECHANICAL CLEANINGAs brieﬂy discussed earlier, there are many types of soil on manufactured products,including organic substances such as oil or inorganic materials such as mineral-typerust inhibitors, scale, or rust. Many of these soils can be effectively removed bymechanically abrading the surface. Mechanical methods, including wire brushing,abrasive blasting, grinding, and sanding, are used to smooth as well as clean surfaces.Mechanical cleaning with a hand-held grinder or a manual blast system can be veryeffective, but it is very labor intensive. In-line blasting can be used to automate theprocess. Mechanical cleaning is sometimes the only way to remove excessive dirt,rust, or scale.18.104.22.168 BlastingBlasting with sand or grit will remove mill scale, rust, or previous coatings from asubstrate and create a surface proﬁle that provides good coating adhesion. The dry ﬁlmthickness of coatings used over a shot-blasted substrate is determined by the proﬁleproduced. A general rule of thumb would be 1 mil over the peaks of the proﬁle.Thicker ﬁlms are recommended, if the part will be used in an outdoor application. Blasting operations can be manual batch systems or automated in-line systems.Blasting systems can use high-pressure nozzles or a centrifugal wheel to deliver theblast media. Nozzle blast systems require compressed air for delivery of the media,while a wheel system uses centrifugal force. Even though the compressed air is anadded cost, it may be necessary to direct nozzles into hard to reach areas of a part.The blast area must be enclosed to contain the blast media and dust. A blasted surface will create a very good anchor pattern for a coating. A blastsystem does not require as much space as a spray washer. Chemical use, mainten-ance, and the associated efﬂuent are avoided. Mechanical treatments may be theonly treatment required for ﬁnishes, where initial coating adhesion is the only crit-ical requirement. However, mechanical cleaning alone will not provide undercoatcorrosion resistance or extend the life of the ﬁnished product. Adequate coveragewith the coating material is critical, if extended life is expected over a blast-onlysurface. The ﬁlm thickness of the coating on a blasted surface must be thick enoughto cover the peaks and valleys of the anchor pattern created by the abrasion. Handheld air-blast systems are very dependent on the concentration of the oper-ator, and the quality may vary. Blast cabinets are often suction-feed systems thatdraw particles into the spray gun by induced vacuum and accelerate the media with ametered stream of compressed air. Pressure-blast systems use a pressurized vessel todeliver the media, providing higher nozzle velocity that can clean the surface muchfaster than a suction system. Blast cabinets function similar to any booth designed for containment of over-sprayed material. Negative pressure within the cabinet is maintained with a fan that
6 Paint Technology Handbookdraws air into the enclosure through a suitable ﬁlter. Typically, this exhaust systemwill use a cyclone separator to remove the dust and ﬁne particles from the airstreamand recover the media for reuse. The scrap material that is separated out of theairstream is collected for disposal in a container attached to a dust collector. Thisscrap material should contain a small percentage of the heavier, reusable media toindicate that the fan pull is sufﬁcient to prevent the buildup of ﬁnes in the recoveredblast media. A vibratory screener can be added to the process to further reﬁne therecovered material and maintain consistent particle size. Turbine-blast systems use high-speed turbine wheel with blades. The media ismetered to the center of the wheel where it is fed onto the blades, which sling theparticles at the surface being blasted. These systems are more energy efﬁcient thanair-blast systems, because they do not use compressed air for delivery. Abrasive blasting is most often used for the preparation of heavy structural parts,particularly HRS welded components. It does an excellent job of removing rust,smut, carbonized oils, and inorganic surface contaminants that are characteristicof this type of product. It can also effectively remove organic soils as long asthe blast media is maintained to avoid a buildup of oil that can cause contamina-tion. The blasting dust needs to be washed away or blown off before the coating isapplied. Different blast media can be used to vary the proﬁle created on the metal surface.Less aggressive media will remove most soils without cutting too deeply into themetal and leaving a visible texture on the metal surface. More aggressive mediacan be used to cut stubborn encrustations, such as red oxides, but it will leave moretexture on the surface. A blast system requires less space than a spray washer that uses chemical clean-ing and it does not generate any wastewater. Mechanical cleaning may be the onlytreatment required for ﬁnishes where initial paint adhesion is required. However,mechanical cleaning alone will not provide undercoat corrosion resistance or extendthe life of the ﬁnished product. The degree of cleaning with the blast operation depends on the qualityrequirements of the surface. Published documents clearly deﬁne quality grades ofblast-cleaned steel surfaces. Pictorial standards were originally developed by theSwedish Corrosion Committee and later adopted by the Steel Structures PaintingCouncil (SSPC) (Table 1.1) and other organizations. The principal four grades ofblasting endorsed by the SSPC are as follows: White metal blast: Removal of all visible rust, mill scale, paint, and foreign matter. Used for conditions where corrosion resistance is very important and the environment is highly corrosive. Near white metal blast: Blast cleaning until at least 95% of all surface area is free of all visible residues. Used for harsh environments where product is exposed to heavy usage. Commercial blast: Blast cleaning until at least two-thirds of the surface is free of all visible residues. For applications where tightly adhering contaminants are allowable on the surface; used for products with lower quality standards and noncorrosive environments.
Part Preparation Processes and Equipment 7 TABLE 1.1 Metal Blast Standards Degree of Cleanliness SSPC Standard NACE Standard White metal blast SSPC-SP 5 NACE No. 1 Near white metal blast SSPC-SP 10 NACE No. 2 Commercial blast SSPC-SP 6 NACE No. 3 Brush of blast SSPC-SP 7 NACE No. 4 For additional information on blast cleaning standards: Plaster, H.J., Blast Cleaning & Allied Processes, Vols. I and II, Industrial Newspapers Ltd., London, 1973 and Fuchs, F.J., “Abrasive Blasting Systems,” in Metal Finishing Guidebook & Directory, Vol. 95, No. 5A, Metal Finishing, Hackensack, NJ, 1997, p. 49. Brush-off cleaning: Blast cleaning of all except tightly adhering residues of mill scale, rust, and old coatings, exposing numerous evenly distributed ﬂecks of underlying metal. Acceptable in noncorrosive environments where long-term coating life is not expected. The Swedish Standards Association (SIS) includes good equivalents of thesestandards. The British Standards Institute (BSI) also includes very close equivalentsof the ﬁrst three of these standards. The National Association of Corrosion Engineers(NACE) has also developed a set of encapsulated steel coupons that simulate the fourdegrees of cleanliness (Table 1.1).22.214.171.124 Blast MediaThe blast media affects the depth of the blast proﬁle and surface roughness afterblasting. Blast media can be made of natural material such as silica, sand, mineralsand, ﬂint, garnet, zircon, and other mineral products. Some natural by-products arealso used for blasting, such as walnut shell or corncob. Other blast materials aremanufactured using a variety of metal and nonmetal compositions such as steel, iron,aluminum oxide, silicon carbide, plastic, wheat starch, and glass bead. The size of the media particles will affect the blast pattern. Other media selectioncriteria include how well it will cut, how well it will recycle, and how much it cost.It is also important to know if there are any health and safety issues, such as lungproblems associated with silica, and if the media will leave by-products on the surface,such as oils from walnut shells. Table 1.2 shows some common blast media and theircomparative characteristics. In addition to the comparative issues listed in Table 1.2, it is a good idea to testdifferent media to have a visual idea of the effect that they will have on the part. Hard grit media such as aluminum oxide will cut faster and deeper than soft,angular media such as plastic or agricultural grit. Mineral, ceramic, or metallic gritmedia are used in air-blast systems. Iron and steel media are more often used inturbine-blast equipment.
8TABLE 1.2Comparison of Blast Media Mesh Density Mohs FriabilityMaterial Size (US) Shape (lb/ft3 ) (Hardness) (Breakdown Factor) Initial Cost No. of Cycles Cost per UseSilica sand 6–270 A, S 100 5.0–6.0 High Low 1 Med.Mineral slag 8–80 A 85–112 7.0–7.5 High Med. 1–2 Med.Steel grit 10–325 A 230 8.0 Low High 200+ Med.Steel shot 8–200 S 280 8.0 Low High 200+ LowAluminum oxide 12–325 A 125 8.0–9.0 Med. High 6–8 Med.Glass bead 10–400 S 85–90 5.5 Med. Med. 8–10 LowPlastic 12–80 A 45–60 3.0–4.0 Low/med. High 8–10 Med.Wheat starch 12–50 A 90 2.8–3.0 High High 10–12 HighCorn cob 8–40 A 35–40 2.0–4.5 Med. Low 4–5 LowA = angular product that cuts more sharply; S = spherical product that peens and does not cut as sharply; Med. = medium. Paint Technology Handbook
Part Preparation Processes and Equipment 9 Materials that are more prone to fracture, reﬂected in the chart by friability, arenot good materials for recycling, because the particle size is reduced during the blastprocess and the media may not be of sufﬁcient size and sharpness to cut soils fromthe surface. The recirculated material will not be as effective, and the surface willvary widely after blasting.126.96.36.199 Vibratory Cleaning or TumblingVibratory systems use an abrasive media in a cleaning solution to remove burrs, roughedges, and surface contamination. They can be useful for preparation of small castingsor parts that have trim die ﬂash or rough edges. They will remove the roughness anddried-on compounds that are often present on a cast surface or the burrs left behindon a sawed edge. Vibratory cleaning will leave some residue on the surface, and it isa good idea to spray clean parts after the vibratory polishing so that and residualcleaning compound is removed before coating.1.1.3 CHEMICAL CLEANINGThe ﬁrst step in the chemical pretreatment process is the removal of dirt, oils, andother soils that could cause surface defects, interfere with the development of agood quality conversion coating, or interfere with paint adhesion. Chemical cleaningmethods include wiping the part with a rag, dipping the part into a solution, or usinga spray cleaning system. The cleaner may be alkaline, acidic, neutral, solvent, oran emulsion. The particular cleaner and process used will depend on the soils to beremoved, the size and substrate material of the part, the type of coating to be applied,and the quality goals for the product.1.1.4 CHEMICAL CLEANING PROCESSESThe different methods of chemical cleaning have certain applications where they ﬁtand limitations that make them unsuitable for other applications. A review of thevarious methods of applying a chemical cleaner helps to understand these strengthsand limitations.188.8.131.52 Hand WipeThe most inexpensive method of cleaning from an equipment perspective is manualcleaning of parts. This would normally involve hand-wiping parts with a solvent oraqueous (water based) cleaning solution. Manual cleaning can be somewhat effectivein terms of soil removal but is very costly in terms of labor and very slow in termsof production time. Because of this, hand-wiping of parts is rarely done except on aspot basis. Hand wiping with a clean cloth does not require any capital investment, but it isnot very effective at soil removal; it has a high labor content, is inconsistent, and maycreate health and safety problems.
10 Paint Technology Handbook184.108.40.206 Immersion CleaningCleaning by immersion in solution is often used for small parts in a batch system.Immersion systems can be either static (still) or agitated. Immersion cycle times aretypically longer than spray cleaning methods, because spray systems have the addedcleaning power of mechanical energy from spray pressure. Systems with no agitationrequire longer cycle times, and they are not as effective. Agitated immersion systems have the added beneﬁt of physical movementbetween the solution and the parts being cleaned. This aids in the overall speed ofreaction taking place between the cleaning compound and the soil. Agitation may beachieved in the tank through air addition or blade mixing. Some dip systems mayalso use a hoist to lift a basket of parts up and down in the tank to provide agitation.Dip systems normally require higher chemical concentration than spray systems andlonger operation times, even with agitation. When the parts are lifted up from the chemical solution, they may retain someresidual chemicals or oil that may ﬂoat to the surface of the solution. Cleaners usedin dip systems should be products designed to emulsify oils rather than products thatdisperse the oils and allow them to ﬂoat to the surface. Many systems use some immersion cleaning along with spray stations.Automotive systems often include some immersion stages to make sure that all ofthe surfaces of the product are fully wetted and dirt is loosened inside and outside ofthe part. The use of immersion with spray stages can enhance overall performance.220.127.116.11 Hand-Held Spray WandHandheld spray wands or steam spray systems are often used to clean parts in abatch powder coating operation. A manual operator has the time to focus attentionon stubborn soils and hard-to-reach areas, providing very thorough removal of soils.Spray wands are often used for larger parts that cannot be easily transported throughautomated systems. The spray wand is used inside a booth. The booth encloses the process so thatthe water vapors is captured and exhausted to atmosphere. Over-sprayed solutioncan be run straight to drain or captured, ﬁltered, and reused. As in manual wiping,this process is time consuming and is not efﬁcient for large numbers of small parts. High-pressure spray wands can use hydraulic pressure as the force to do thecleaning. This type of cleaning is done at pressures ranging from 400 to 1000 psi. Thetemperature ranges from cold water to hot water (200◦ F) for high-pressure washing.This type of washing is done with or without cleaning compounds. The water volumeused ranges from 2 to 35 gal/min. Steam generators are sometimes used to produce dry saturated steam for spraycleaning. In a coil-type, forced-circulation steam generator, water is forced into thecoil toward the discharge point. As the water passes through the coil, it becomesprogressively hotter as steam is formed. Most of the water is evaporated before it dis-charges into the steam generator. This type of steam generator is designed to circulatemore water than is evaporated. This excess water carries loose scale particles andother foreign matter through the coil and into the separator. Here, the water and scaleparticles are separated from the steam, providing high-quality, dry, saturated steam.
Part Preparation Processes and Equipment 11 Steam systems are not as effective as hot-water systems. They do not provideas much energy at the parts surface and do not wet out the surface as well. The energyrequired to generate steam is higher than the hot-water systems. Spray wand systems provide ﬂexibility for contact time and angle and the highpressure can remove heavy greases. Higher foaming surfactants may be used, becausefoam is generally not a concern and higher temperatures are possible, so it may beeasier to melt waxes and grease. The labor content and the chemical cost are high. Cycle times are long, and spraywands are not suitable for higher volumes of small parts. Spray wands do not offerthe wide variety of chemicals and process steps that are possible with multistage spraywashers.18.104.22.168 Ultrasonic CleaningUltrasonic cleaning utilizes high-frequency sound waves to increase the effective-ness of the cleaning chemicals and the agitation at the soil–substrate interface onthe material. Transducers are located either inside or outside the cleaning vessel toproduce the sound waves. When the sound waves reach the surface of the materialto be cleaned, they cause cavitation. Cavitation is the formation and collapse ofvapor bubbles and voids in liquid by acoustic energy at high frequencies. These tinyexploding bubbles act as a brush to carry particles and used chemical away from thesurface of the substrate. This increases the capabilities of the chemicals by continu-ously replacing inactive, reacted product, with fresh chemical. In addition, it gives thechemicals new sites to work on by breaking away loose dirt and other contaminants. Metals are the best candidates for ultrasonic cleaning, since their crystallinemolecular structure allows vibration to occur relatively freely. Rubbers and plasticsdo not work nearly as well, because the molecular structure of these materials is morelikely to absorb the shock waves rather than vibrate with them. Ultrasonic cleaning works very well for cleaning metal surfaces and they aremultimetal safe. Complex geometries and blind holes do not diminish the effective-ness of the sound waves since they clean the part throughout; these are not line-of-sitedevices. The consistency of ultrasonic cleaning is much higher than conventionalcleaning methods as well. Cleaning occurs on all surfaces of the object for the entireduration of the process. Ultrasonic is particularly effective for some porous metalssuch as bronze. Larger loads do not clean, as well as smaller loads, given the same time frame,due to energy absorption. Large, heavy parts can block each other out and cause poorcleaning.22.214.171.124 Recirculating Spray WashersSpray washers are the most common way to chemically clean and treat a part forapplication of a coating. A spray washer uses a series of spray stages that featuredifferent solutions for different tasks. Each stage of a spray washer consists of thesolution tank, the recirculating pump, plumbing for delivery of the solution, a tankheating system, and the gauges and controls that operate the system. A tunnel ismounted over the tanks to contain the spray process. Parts are usually transported
12 Paint Technology Handbook Spray Tunnel risers Gauges Spray Pump nozzles Overflow Tank Drain Elevation view End view Profile plate Tank Pressure valve access lid Plan viewFIGURE 1.2 Spray washer components.through the washer tunnel on an overhead conveyor, although smaller parts washersmay use a belt-type conveyor. The cleaning solution is recirculated through the sprayheader up to the risers and out through nozzles onto the parts. The parts of the spraywasher are shown in Figure 1.2. The nozzles on the risers aid in the cleaning process by providing a directedpressure spray in a predetermined pattern to completely cover the part. The most com-mon nozzle used in this application is the vee-jet, which produces a ﬂat, fan-shapedspray of uniform density. The angle of spray (20◦ –90◦ ) is determined by the nozzleand riser spacing in the washer stage and the desired level of overlap in the spraypattern. As seen in Figure 1.2, the nozzles are placed so that all surfaces of the partare reached as it proceeds through each of the various stages. The recirculating spray washer is the most efﬁcient process for continuousproduction ﬂows. It can handle large volumes of products and provide excellentcleaning and treatment of most parts. Spray washers are signiﬁcantly more expensive than manual cleaning methodsand they also cost more to operate. They require more maintenance and control toperform properly. The number of stages of a spray washer depends on the substrates to be processed,the type of cleaning and other processes that will be used, space availability, and cost.The end use of the part and the performance requirements of the coating will alsoimpact the number of stages. Generally speaking, more stages will improve cleaningand ﬁnish performance. Three-stage washers are common for products that do not need exceptional cor-rosion resistance. The ﬁrst stage is normally a cleaner or cleaner/conversion coatingfollowed by two rinse stages. The rinse stages are usually recirculated water rinses
Part Preparation Processes and Equipment 13with a volume of water (typically 3–5 gal) overﬂowed to drain and made-up withfresh water to maintain relatively clean rinse water. The cleaner stage is usuallyheated to enhance the performance of the cleaning solution. Rinses are not typicallyheated, although the ﬁnal rinse is sometimes heated to leave the part surface warmand accelerate drying after wash. Stepping up from three stages of pretreatment to ﬁve stages allows the separationof the cleaning and the conversion coating steps, with a rinse in between each pro-cess to reduce cross-contamination of the cleaner and conversion coating solutions.As washers increase in complexity from ﬁve- to seven-stage systems, the added stagesare generally additional cleaners or rinse tanks. Good cleaning is an essential part ofthe pretreatment process. Excellent rinsing ensures that the residual chemicals andsoils are removed before the coating is applied. Proper cleaning of some parts may require a combination of spray and immersionstages. The spray stage combines the chemical properties of the cleaner with theimpingement action of the solution applied under pressure. Immersion penetratesareas of the part that may be inaccessible to the spray and improves wetting of hardto reach surfaces.1.1.5 COMMON INDUSTRIAL CHEMICAL CLEANERSThe selection of the correct chemical product for an application is critical to theproper operation of the cleaning system. Products typically used in pretreatmentinclude alkaline cleaners, neutral cleaners (which also act as detergent additives),acid cleaners, and solvent emulsion cleaners. In each group, there are speciﬁc attrib-utes to be considered. The cleaner selected must have the ability to remove a widevariety of soils, prevent redeposition, provide cleaning even when contaminated,provide foam control, be easily rinsed, and be cost effective. Cleaners are often classiﬁed according to their pH. The pH of the solution isa measurement of the relative alkalinity or acidity. On the pH scale, pure water isneutral and has a pH of 7. A pH below 7 is considered acidic and above 7 is alkaline.Caustic soda has a pH of 13 or 14, while hydrochloric acid has a pH of less than 1.A typical range of pH is shown below. • Alkaline cleaners—mild, pH 9–10.5 — medium, pH 10.5–11.5 — high, pH > 11.5 • Neutral cleaners—pH 6.5–9 • Acid cleaners—pH 1.0–5.5The various components that are used to build an industrial cleaner have their ownunique mechanisms that affect certain soils.126.96.36.199 Alkaline CleaningAlkaline cleaners are popular for metal cleaning operations, primarily because ofthe versatility of their components and their ability to break down organic soils.